Composition profiling of inhomogeneous SiGe nanostructures by Raman spectroscopy
 Andrea Picco^{1},
 Emiliano Bonera^{1}Email author,
 Fabio Pezzoli^{1, 2},
 Emanuele Grilli^{1},
 Oliver G Schmidt^{2},
 Fabio Isa^{3},
 Stefano Cecchi^{3} and
 Mario Guzzi^{1}
DOI: 10.1186/1556276X7633
© Picco et al.; licensee Springer. 2012
Received: 8 August 2012
Accepted: 1 November 2012
Published: 21 November 2012
Abstract
In this work, we present an experimental procedure to measure the composition distribution within inhomogeneous SiGe nanostructures. The method is based on the Raman spectra of the nanostructures, quantitatively analyzed through the knowledge of the scattering efficiency of SiGe as a function of composition and excitation wavelength. The accuracy of the method and its limitations are evidenced through the analysis of a multilayer and of selfassembled islands.
Keywords
Raman SiGe Nanotechnology Composition Structural characterization Raman efficiencyBackground
SiGe nanostructures[1] such as quantum dots and islands are appealing for applications in photonics[2], microelectronics[3], thermoelectrics[4], and possibly quantum computation[5]. The fabrication of these nanostructures is often accompanied by composition inhomogeneities, as in the case of StranskiKrastanov grown selfassembled islands[6]. The composition profile is a crucial parameter for several functional properties, such as bandgap and mobility. This has boosted the need of techniques to gather access to the exact SiGe concentration profiles. Ge distribution within the nanostructures can be measured by transmission electron microscopy (TEM)[7], atomic force microscopy (AFM)based nanotomography[8, 9], and Xray diffraction[6, 10]. Raman spectroscopy is a commonly used technique for the structural characterization of homogeneous SiGe[11–14], and in this work, we demonstrate how it is possible to extend its capabilities to the extraction of compositional profiles, with the advantage over the aforementioned techniques of being simultaneously fast and nondestructive.
The Raman spectrum of SiGe (Si_{1−x}Ge_{ x }) depends on the relative alloy Ge content x. Three Raman peaks can be observed and related to SiSi, SiGe, and GeGe vibrations: their relative intensity and frequency are functions of x. The Raman spectrum Ф of an inhomogeneous structure contains information about the internal composition profile, i.e., Ф is a convolution between the composition profile and a set of Raman spectra, ϕ_{ x }, of bulk SiGe alloys with constant composition x. The Raman spectra set, ϕ_{ x }, represents the amplitude of scattering as a function of the wave number. The convolution is weighted by the spatial distribution of the excitation light in the nanostructures, the collection geometry, as well as by S_{ x }, the Raman efficiency of the alloy, which is also dependent on x for a given excitation wavelength λ_{exc}.[15]. We want to show that the Raman spectrum can be used to reconstruct the spatial distribution of composition within an inhomogeneous sample, a process which was not possible before the recent publication of the values of S_{ x } in the work of Picco et al.[15].
We will present a procedure for individuating the different compositions contributing to Ф and also for the reconstruction of a composition profile. First, the method will be discussed in detail while being applied to a SiGe multilayer. The choice of this sample was based on the fact that it can be characterized precisely with other experimental procedures and therefore can represent the best benchmark for the determination of the method’s validity. After a detailed discussion on the multilayer, the procedure will be also applied to SiGe selfassembled nanoislands.
Methods
Raman spectra were acquired with a Jasco R800 doubleadditive spectrometer (Jasco Corporation, Tokyo, Japan) coupled to a microscope. All the spectra were acquired with an excitation wavelength, λ_{exc} = 532 nm. Notch filters were used to reduce the radiation at the same wavelength of λ_{exc}. The resolution of the instrument was about 0.6 cm^{−1}, a negligible value as compared to the natural bandwidth of all the Raman phonons at any composition. The spatial resolution achieved with an objective with a numerical aperture of 0.75 was about 1 μm. The incident power density was kept at less than 0.1 mW/μm^{2} in order to prevent the sample from heating (this value was determined by observing that lower powers did not modify the spectrum).
Results and discussion
Deconvolution of the Raman spectrum of the SiGe multilayer
The determination of the spectral contributions a_{ x } consists in a deconvolution of the experimental spectrum, Ф, and represents an important added value with respect to the methods based on Raman spectroscopy found in previous works[12, 17] where one must rely on the assumption to have a homogeneous sample. The set of a_{ x } unfolds the presence of a distribution of compositions within the probed layer. In addition, the knowledge of a_{ x } can be also the starting point for a reconstruction of the composition profile. We will demonstrate these features by analyzing a SiGe multilayer and SiGe selfassembled islands.
The deconvolution must be carried out starting from a set of ϕ_{ x } that can be measured or taken from the work of Picco et al.[15]. The starting point of the procedure is a choice of a basis formed by a limited number of ϕ_{ x } and therefore a relatively high value of Δx. At this point, whatever the initial seeds, a_{ x }, the algorithm always converges to the same unique solution. The next step is to decrease Δx, and therefore to increase the number of ϕ_{ x }, and repeat the algorithm. The process continues as long as shrinking Δx leads to a decrease of Δ_{1}, and the solution keeps on being unique. When the uniqueness condition is not satisfied, the solution of the algorithm is discarded, and the process ends. In the example reported here, we obtained the best spectrum with a unique solution using 21 ϕ_{ x } spectra with a sampling interval Δx of 0.05. The minimization of Equation 1 leads to the generation of a reconstructed spectrum Σa_{ x }ϕ_{ x } (Figure 1a, upper red spectrum) which most closely approximates Ф. The inspection of the a_{ x } values shows that the spectrum has contributions from compositions around [0.20 to 0.25], [0.40 to 0.45], [0.55 to 0.65], and [0.75 to 0.95], as shown in Figure 1b. These x values are in agreement with the nominal values of composition within an accuracy Δx ≈ 0.10, a figure that demonstrates the potential of this kind of analysis.
Notice that there are some limitations to the applicability of this procedure. This method cannot work in those nanostructures where a strong phonon confinement takes place, typically with dimensions of a few nanometers. In all other cases, the main problems related to the determination of a_{ x } rise from mechanical strain. Since the ϕ_{ x } spectra are acquired from unstrained bulk, the effect of strain on Ф cannot be taken into account from Equation 1. The small discrepancies in Figure 1a are indeed related to the small residual strain in the stack. Other works in the literature[12] show, for example, that a biaxial strain of the order of 1% modifies the spectral position of the SiSi band like a change in x of about 10%. In this sample, we checked the residual strain by Xray diffraction in the layers (+0.3%, +0.1%, +0.1%, and −0.1% from top to bottom); therefore, the success of the deconvolution of Figure 1 relies in the fact that the strain was small enough not to corrupt significantly the analysis. It is important to underline that Figure 1b was obtained from one single spectrum and shows clearly that Ф is a superposition of several contributions, shedding light on Ge inhomogeneous distributions in the sample: a result which is beyond the grasp of the optical methods reported in the literature.
Composition profiling of the SiGe multilayer
where it must be summed up for all the layers x′ above the layer x so that e^{− 2m} represents the attenuation of the excitation and collection for the buried layer x. The minimization of Equation 2 leads to the determination of d_{ x }. In this part of the procedure, the main source of error is the knowledge of L_{ x }, especially for the buried layers, where this uncertainty is more relevant. This can be observed, for example, by plotting a spectrum reconstructed from the d_{ x } values obtained by SEM (Figure 1a, lower red spectrum), while the SiSi and SiGe modes are well reproduced because they are generated mostly by the upper layers; the simulation of the GeGe mode is not accurate since it is generated by the lower buried layers. In addition, the condition d_{ x } >> L_{ x } must be false for all the layers involved in the simulation, i.e., each layer must be properly excited by the laser throughout all its thickness, and this represents another possible limitation of the technique. In this sample, the deepest layer did not satisfy this condition and was excluded from the minimization. The results are reported in Figure 1c (red line). During minimization, we fixed the total thickness of the stack d_{stack} and imposed that Gericher layers were below Siricher layers. Within the region of the sample involved in the simulation, for each value of the vertical position z, the composition profile obtained with the Raman analysis matches the profile independently measured by SEM (Figure 1c, black) within the remarkable accuracy of 10%.
SiGe nanoislands
In order to test its validity on different structures, we applied this method to the case of selfassembled SiGe islands grown by StranskiKrastanov process on a flat Si(001) substrate. The experimental spectrum of the islands, as shown in Figure 2a, was analyzed with Equation 1. Each island is treated as a stack of SiGe homogeneous disks. The signal from the substrate is excluded from the algorithm. Contributions of compositions between 0.25 and 0.50 are detected, with two major components at 0.35 and 0.45, as shown in Figure 2b, indicating a quite homogeneous inner composition. In addition to the deconvolution, we tried to get a coarse indication of the vertical profile of x by approximating a SiGe island as a multilayer stack with high Ge content on top (therefore neglecting a lateral variation of composition). The composition profile was obtained through the minimization of Equation 2 with the only constraint on the total thickness given by the AFM profile. The results in Figure 2b show values of x which are compatible with those results that one expects are from islands grown at similar temperatures[18]. By comparison with the results in the literature[18], we observe that despite the roughness of the approximation within the islands, the vertical distribution of x is in agreement with the trend observed with other techniques. Furthermore, Figure 2c shows that in this experiment the effect of strain cannot introduce an artifact in the determination of the composition of more than 0.10. We underline that the profile was obtained with a nondestructive measurement from one single spectrum.
Conclusions
In conclusion, we presented a procedure for the analysis of the Raman spectra of inhomogeneous SiGe samples. This procedure is not intended to replace other techniques such as Xray or TEM, but rather, it intends to offer a fast and nondestructive alternative for the investigation of several different nanostructures with a diffractionlimited spatial resolution, with the possibility of investigating single isolated nanostructures. This procedure is able to detect the composition values present in the sample and can also give a composition profile of the structure. While other methods based on Raman spectroscopy require the assumption of a homogeneous structure and can measure simultaneously composition and strain, this method can measure composition inhomogeneity, but its main requirement is a low mechanical strain. We also analyzed the other possible errors and limitations due to confinement, opacity of the layers, and uncertainty in the knowledge of the optical functions. The validity and the limitations of the method were tested with the aid of a multilayer stack independently characterized with other techniques. The application of this procedure to the study of selfassembled SiGe islands yields results in agreement with those from other techniques available in the literature. The method can be effective in SiGe nanotechnology especially when it is necessary to face high yields of samples, and it can be applied to the structural characterization of any kind of nanostructures such as quantum wells, islands, nanowires, or nanocrystals.
Endnote
^{a}The minimization procedure can be carried out by commercially available routines, e.g., the implementation of the nonnegative least square problem minimization algorithm available in Matlab.
Abbreviations
 AFM:

Atomic force microscopy
 SEM:

Scanning electron microscopy
 TEM:

Transmission electron microscopy.
Declarations
Acknowledgments
The authors acknowledge G Isella (LNESS Como, Italy) and CV Falub (ETH Zurich, Switzerland). F Pezzoli was supported by Regione Lombardia through “Dote Ricercatori”. Financial support was provided by Fondazione Cariplo, DefCon4 Project, grant 2011–0331, and partially from the EU project dDotFET no. 012150. We thank M Stoffel for useful discussions.
Authors’ Affiliations
References
 Pezzoli F, Deneke CH, Schmidt OG: Strain engineering of silicongermanium (SiGe) micro and nanostructures. In SiliconGermanium (SiGe) Nanostructures: Production, Properties, and Applications in Electronics, Chapter 11. Edited by: Shiraki Y, Usami N. Cambridge: Woodhead Publishing; 2011.
 Tsybeskov L, Lockwood DJ: Silicongermanium nanostructures for light emitters and onchip optical interconnects. Proceedings of the IEEE 2009, 97: 1284.View Article
 Schmidt OG, Eberl K: Selfassembled Ge/Si dots for faster field effect transistors. IEEE Trans Elec Dev 2001, 48: 1175. 10.1109/16.925244View Article
 Pernot G, Stoffel M, Savic I, Pezzoli F, Chen P: Precise control of thermal conductivity at the nanoscale through individual phononscattering barriers. Nat Mater 2010, 9: 491. 10.1038/nmat2752View Article
 Katsaros G, Spathis P, Stoffel M, Fournel F, Mongillo M, Bouchiat V, Lefloch F, Rastelli A, Schmidt OG, De Franceschi S: Hybrid superconductorsemiconductor devices made from selfassembled SiGe nanocrystals on silicon. Nat Nanotechnol 2010, 5: 458. 10.1038/nnano.2010.84View Article
 Stangl J, Holý V, Bauer G: Structural properties of selforganized semiconductor nanostructures. Rev Mod Phys 2004, 76: 725. 10.1103/RevModPhys.76.725View Article
 Floyd M, Zhang YT, Driver KP, Drucker J, Crozier PA, Smith DJ: Nanometerscale composition measurements of Ge/Si(100) islands. Appl Phys Lett 2003, 82: 1473. 10.1063/1.1558215View Article
 Rastelli A, Stoffel M, Merdzhanova T, Schmidt OG: Intermixing and composition profiles of strained SiGe islands on Si(001). J Phys Condens Matter 2008, 20: 454214. 10.1088/09538984/20/45/454214View Article
 Pezzoli F, Stoffel M, Merdzhanova T, Rastelli A, Schmidt OG: Alloying and strain relaxation in SiGe islands grown on pitpatterned Si(001) substrates probed by nanotomography. Nanoscale Res Lett 2009, 4: 1073. 10.1007/s1167100993604View Article
 Schülli TU, Stangl J, Zhong Z, Lechner RT, Sztucki M, Metzger TH, Bauer G: Direct determination of strain and composition profiles in SiGe islands by anomalous Xray diffraction at high momentum transfer. Phys Rev Lett 2003, 90: 066105.View Article
 Mooney PM, Dacol FH, Tsang JC, Chu JO: Raman scattering analysis of relaxed GexSi1−x alloy layers. Appl Phys Lett 2069, 1993: 62.
 Pezzoli F, Bonera E, Grilli E, Guzzi M, Sanguinetti S, Chrastina D, Isella G, von Känel H, Wintersberger E, Stangl J, Bauer G: Raman spectroscopy determination of composition and strain in Si1−xGex/Si heterostructures. Mat Sci Semicond Proc. 2008, 11: 279. 10.1016/j.mssp.2008.09.012View Article
 Pezzoli F, Bonera E, Grilli E, Guzzi M, Sanguinetti S, Chrastina D, Isella G, von Känel H, Wintersberger E, Stangl J, Bauer G: Phonon strain shift coefficients in Si1−xGex alloys. J Appl Phys 2008, 103: 093521. 10.1063/1.2913052View Article
 Bonera E, Pezzoli F, Picco A, Vastola G, Stoffel M, Grilli E, Guzzi M, Rastelli A, Schmidt OG, Miglio L: Strain in a single ultrathin silicon layer on top of SiGe islands: Raman spectroscopy and simulations. Phys Rev B 2009, 79: 075321.View Article
 Picco A, Bonera E, Grilli E, Guzzi M, Giarola M, Mariotto G, Chrastina D, Isella G: Raman efficiency in SiGe alloys. Phys Rev B 2010, 82: 115317.View Article
 Stoffel M, Rastelli A, Tersoff J, Merdzhanova T, Schmidt OG: Local equilibrium and global relaxation of strained SiGe∕Si(001) layers. Phys Rev B 2006, 74: 155326.View Article
 Palik ED: Handbook of Optical Constants of Solids II. 7th edition. Waltham: Academic Press; 1998.
 Rastelli A, Stoffel M, Malachias A, Merdzhanova T, Katsaros G, Kern K, Metzger TH, Schmidt OG: Threedimensional composition profiles of single quantum dots determined by scanningprobemicroscopybased nanotomography. Nano Lett 2008, 8: 1404. 10.1021/nl080290yView Article
Copyright
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.